# Simulation Study on Friction and Wear Law of Brake Pad in High-Power Disc Brake

Authors: S. Zhang; Q. Hao; Y. Liu; L. Jin; F. Ma; Z. Sha; D. Yang
Journal: Mathematical Problems in Engineering
 (2019)

---

## Abstract

For the serious and uneven wear of the brake pad in the high-power disc brake during braking, the dynamic variation of the brake disc and the brake pad interface variable is considered, the wear calculation model is established based on the friction and wear mechanism, and the wear depth and volume of the brake pad can be calculated by equations. A finite element model of the brake disc and the brake pad is established by DEFORM software which can analyze wear of the brake pad directly. The variation trend of wear during braking is studied, and influences of braking load and initial braking speed on the wear are analyzed. The results show that the amount of the wear increases rapidly in the early wear stage of braking, and it becomes slow in the later stage; the wear of the brake pad is serious at the friction inlet and outlet, and the middle area of the brake pad is lightly worn; heavy braking load and high initial braking speed can exacerbate the wear of the brake pad.


---

## Body

## 1. Introduction

Disc brakes are widely used in aircrafts, automobiles, cranes, wind turbines, and other mechanical equipments, and it is a significant component to ensure the operation safety of machine. Because of the advantages of stable braking performance and large torque capacity, the disc brake has become one of the most advanced brake devices. Under high-power emergency braking condition, the disc brake is used to stop the high-speed brake disc with heavy load. During the entire braking process, a large amount of friction heat is generated by the friction effect of the brake disc and pad, resulting in heat fade and thermal damage on the brake pad [1]. A small part of friction heat is stored in friction material as internal energy. Deformation and wear of material could occur on the brake pad because of uneven distribution of the large amount of heat. The friction heat causes localized high temperature of contact surface and uneven thermal deformation of the brake pad. These above result in an uneven distribution of the contact stress between the brake disc and pad. Because of the braking performance degradation corresponding to the variation of the wear condition of the brake disc and pad, friction and wear analysis of high-power disc brake has become a research hotspot all over the world.Friction heat distributes unevenly due to various reasons, such as thermal expansion and geometrical defects. It is well known that thermoelastic distortion affects the contact stress distribution and leads to thermoelastic instability, or where the contact stress is concentrated in one or more small regions on the brake disc surface. These regions then get very high temperatures with low frequency vibration. Disc thickness variation will further promote the localized contact. Nonuniform contact can also be generated by disc lateral runout. Lee et al. investigated the effects of various contact conditions on the heating patterns and judder characteristics of a disc brake. The baseline friction material used in the study was modified based on the theory of thermoelastic instability and dynamometer testing [2]. Then, numerical techniques had been developed to characterize the contact temperature problem of composite materials, and the contact temperature distribution between real composite-steel surfaces could be evaluated in sliding contact [3]. Therefore, some researchers examined finite element models for studying the friction heat of the disc brake to obtain the temperature distribution and the thermal and residual stresses [4–6].The generation of friction heat is affected by the braking conditions, determined by the braking parameters. The braking parameters have a major impact on the wear. Yevtushenko et al. studied the numerical simulation of frictional heating in a disc brake of a typical passenger vehicle based on the equation of motion and the boundary-value problem of heat conduction. An influence of temperature-dependent coefficient of friction on the braking parameters was studied [7]. Sergienko et al. studied a dimensionless heat problem for a friction pair of a multidisc brake under conditions of a linear decrease in the friction power of discs with time. Thermal state of friction pairs of the multidisc brake under load and velocity conditions of the friction of the discs that simulate service braking of a wheel tractor was experimentally and theoretically studied [8]. Accounting for the initial decrease and the subsequent increase in the frictional forces with increasing relative velocity, Kaliyannan et al. considered a negative gradient friction model and obtained approximate analytical expressions for the amplitudes and base frequencies of friction-induced stick-slip and pure-slip phases of oscillations [9]. Liu et al. proposed an iterative integration method to analyze parametric instabilities and compared with an established numerical method. The impacts of friction coefficient, bending effect, contact ratio, and modal damping on the stability boundaries were revealed [10]. Rezaei et al. employed an adaptive wear modeling method to study the wear progress in radial sliding bearings contacting with a rotary shaft.In the developed wear processor algorithm, remeshing not only was performed on the contact elements but also was executed for their proximity elements. The simulations also demonstrated how the contact pressure evolved during the wear process and how the clearance influenced this evolution [11]. Bortoleto et al. presented a computational study based on the linear Archard’s wear law and finite element modeling (FEM), in order to analyze unlubricated sliding wear observed in typical pin on disc tests. Such modeling was developed by using ABAQUS software with 3D deformable geometries and elastic-plastic material behavior for the contact surfaces. Numerical and experimental results were compared in terms of wear rate and friction coefficient. In the numerical simulation, the stress field distribution and changes in the surface profile across the worn track of the disc were analyzed [12]. Lamjahdy et al. measured the erosion rate of the brake disc and pad, depending on temperature changes and deformation by performing experiments and simulations at varying velocities and load conditions. Relationships between erosion rates and temperature changes for different brake disc velocities and load conditions were investigated [13]. Baldari et al. investigated the numerical simulation method of thermal load, contact stress, and wear coupling behavior between the brake disc and pad. And the wear behavior of the brake pad in both stress-wear coupled and emergency braking conditions was simulated respectively [14]. Zhang et al. based their study on the pin-disc wear test and the thermal-stress-wear sequential coupling method, considering influence of temperature on the friction pair material obtained in the evolution process of temperature field, stress field, and wear amount [15].To study the friction and wear of the brake disc and pad, mathematical equations were used to calculate the wear depth. Because the change element of materials in finite element software is difficult to achieve, there is a certain limitation on the calculation of wear depth and the expression of wear profile by the software of ANSYS and ABAQUS. However, this paper calculates the wear depth by considering the factors affecting wear. Based on the tribological principle of the high-power disc brake, the friction and wear characteristics of the brake pad under high-speed and heavy-load conditions are studied, and the influence of braking parameters on the wear of the brake pad is analyzed.


## 2. Analysis of Friction and Wear Mechanism of the Brake Pad

The wear of the brake pad is the material damage, and it appears on the surface layer and subsurface layer caused by the thermomechanical coupling effect of the brake friction pair contact surface. It is essentially a complex dynamic changing process, as shown in Figure1. Due to the large difference in hardness of the brake disc and pad, and the effect of the third body hard particles in the contact gap, the mainly wear type is abrasive wear. Abrasive wear can arise from the penetration and plowing out of material forming a surface of hard particles of the brake disc. Meanwhile, the adhesive wear occurs in high temperature regions. Adhesive wear occurs at the starting point for a wear process developing between two conforming friction surfaces. And the wear process cannot be generally characterized by a single type of event, except perhaps in the case of continuous severe wear [16].Figure 1
Diagram of the brake disc and pad wear.The abrasive wear of the brake pad is mainly manifested as “plowing effect”. The large hardness particles or microbulges penetrate and scrape the brake pad material; wear scar and abrasive dust are produced on the surface. The hard particles are pressed into the contact surface of the friction pair under load generating indentation, which increases the surface roughness of the friction pair, so that the contact peak of the microbulge is more likely to form a bond point, and the adhesive wear of the brake pad occurs. Especially under high-speed and heavy-load conditions, due to the large plastic deformation of the contact peak and high surface temperature, the phenomena of the shear in the bond point of fracture are caused by the relative sliding of the brake friction pair surface. A part of shedding materials becomes abrasive dust; others migrate from the brake surface to the disc surface to wear continually.


## 3. Mathematical Model of the Brake Pad Wear

### 3.1. Calculation Model of the Brake Pad Wear

Due to extrusion and friction, the high temperature occurs on the friction pair at high-speed and heavy-load conditions, and there is serious wear on the friction contact. In 1953, the classical Archard wear theory was proposed by J. Archard [17]. The calculation equation is as follows:(1)V=KP·LHwhereV is the wear volume;P is the normal force of the contact surface;L is the relative sliding distance;H is the material hardness;K is the dimensionless wear coefficient. When the time increment is infinitesimal as dt, (1) can be extended to the differential form:(2)dVdL=K·PtHwhere dV is the instantaneous wear volume increment, dL is the instantaneous sliding distance, and Pt is the instantaneous normal interface contact force. Assuming that the wear depth increment on the microelement area ΔA is dh at time dt, the instantaneous wear volume increment can be expressed as(3)dV=ΔAdhwhere ΔA is the contact area of the brake disc and pad.Substituting (3) into (2), and it can be expressed as(4)dhdL=K·pHwhere p is the contact pressure at the contact microelement area ΔA, p=Pt/ΔA. Since the relative sliding distance L is the integral of the speed versus v timet, (4) can be rewritten as(5)dh=K·p·vHdt where the independent variables p and v of theoretical calculation are usually constant.However, under the actual high-speed and heavy-load braking conditions, the contact surface of any friction pair is rough. The actual contact area is related to the micromorphology of the contact surface. The stress value of every node on the contact interface is closely related to the wear depth and wear state of contact surface. The stress value changes with the wear depth change of each node on the contact surface, leading to the change wear degree of contact surface. Similarly, the high speed aggravates the friction of the contact pair, and a large amount of frictional heat is generated, and the friction material structure is changed, so does the hardness. The relationship between hardness and temperature of the material is as follows [18]:(6)H=const·exp⁡αθwhere α is a constant and θ is contact temperature.Wear is affected by the hardness of the friction material, and the change of temperature could affect the hardness of the friction material. Especially under high-speed and heavy-load braking conditions, the change of temperature is an important factor. Simultaneously, the virtual simulation software needs to calculate the relative contact speed, pressure, and temperature. However, the wear factors are considered distance, pressure, and material hardness in the original Archard wear calculation model. Therefore, the classical Archard wear model is no longer applicable for the simulated wear depth of a certain contact node. The Archard model is modified according to actual braking process. The contact pressurept, relative sliding velocity vt, and interface contact temperature θt are considered as influencing factors. The specific correction equation is as follows:(7)dht=K·pt·vtconst·exp⁡α/θtdtThe classical Archard wear equation is usually used to calculate the wear value of the relative rectilinear motion of two objects. However, when the brake disc and the brake pad of high-power disc brake are worn, the brake disc is in a state of rotation. The relative sliding speed of the contact interface is the tangential speed. Decompose the relative sliding tangential velocity:(8)vt=ωt·rwhere ωt is the relative sliding angular velocity and r is the friction radius of the brake pad. Substituting (8) into (7), it can be expressed as (9)dht=K·pt·ωtconst·exp⁡α/θt·rdtThe integral of (9) for time t in one braking time (0,t0) is expressed as(10)ht=K·r·∫0t0pt·ωtconst·exp⁡α/θtdtEquation (10) is a continuous integral solution. However, finite element analysis requires step-by-step solution in virtual simulation. So, the solution of (10) is very difficult because the variable curve of the contact node is very complicated. For the convenience of calculation, the continuous wear value is discretized by the discrete method: a finite small-time increment Δt is selected, and the corresponding wear depth increment is Δh. It is considered that the contact pressure pt, relative sliding angular velocity ωt, and contact temperature θt do not change large during time increment Δt, and the instantaneous values of pt, ωt, and θt are taken; then, Equation (9) becomes(11)Δht=K·r·pt·ωtconst·exp⁡α/θt·ΔtSince the wear of the brake interface is not evenly distributed between the brake disc and pad, the wear volume of the brake pad is solved by discrete method.As shown in Figure2, assuming that the unit friction radius increment is Δr within the time increment Δt, the unit microelement wear area can be expressed as(12)δAt=πr+Δr2-πr2·Δφ2πwhere Δφ is radians increment, Δφ=ωt·Δt. The unit wear volume of the brake pad within the time increment Δt is(13)ΔVt=δAt·ΔhtFigure 2
Calculation model of microelement wear area of the brake pad.Substituting (11) and (12) into (13), it can be expressed as(14)ΔVt=K·Δr+2r·r·Δr2·pt·ωt2const·exp⁡α/θt·Δt2When the disc brake is braking, the brake pad is considered as stationary state. There is wear on the brake pad, and the wear depth increment isΔh in Δt on the unit microelement contact area δA. The brake interface has different wear degrees with the change of the friction factor, and there is a feedback on the friction factor that the wear causes a change in the contact condition. The Euler integral method is used to calculate the wear by computer. The Euler method is a method of changing the differential equation of continuous variables to the difference equation of discrete variables. The numerical calculation is simple and easy, and the numerical convergence is good.In time incrementΔt, the contact pressure pt, relative sliding angular velocity ωt, and contact temperature θt are assumed to be constant. The wear depth increment Δht is obtained by Equation (11). The values of interface contact pressure pt, relative sliding angular velocity ωt, and contact temperature θt after wear can be obtained by the finite element method. Then the wear depth Δht can be calculated and the geometric mode is changed. Such loop iterations calculating the final accumulated wear value of the brake pad wear are obtained. The calculation method is as follows.Assuming that the contact node of the brake disc and the brake pad isi, i=1,2,…,N, and the integral step of the explicit Euler integral isj,j=1,2,…,M, then the contact pressure is pt(i,j), the relative sliding angular velocity is ωt(i,j), the contact temperature is θt(i,j), the wear depth is Δht(i,j), and the wear volume is ΔVt(i,j). The total wear depth h(i,j) and volume V(i,j) of braking at once of the brake pad can be expressed as(15)hi,j=∑j=1mΔht(16)Vi,j=∑j=1mΔVtThen the wear volume of the brake pad during the single braking of the disc brake can be expressed as(17)V=∑i=1nVi,jAccording to (17), the quantitative results of the brake pad wear after braking can be obtained. The process consists of two parts: one is to intercept and output the speed, stress, and temperature data in the wear stage from the time history curves of the contact point; the other is to divide the speed, stress, and temperature data and substitute these data into the equations to solve, as shown in Figure 3. DEFORM software has a special command to control the calculation of wear depth. Equation (5) can be added to the simulation program by compiling method to calculate the wear depth.Figure 3
Flow chart of wear calculation.


### 3.2. Determination of Wear Direction on Brake Pad Node

Affected by friction parameters, the surface roughness of contact surface after braking is different. There are two cases of the brake disc and the brake pad contact node: the boundary node at the edge of the contact surface and the nonboundary node located inside the contact surface. The wear direction of the nonboundary node can be determined by the normal of the contact node, and the wear direction of the boundary node is along the surface of the wear object. For the structured mesh, the connecting line direction of the nodes corresponding to their thickness direction is taken as the wear direction of point. As shown in Figure4, the wear contact area is indicated by dashed line, the nodes 2, 3, 4, and 5 are in the contact area, node 1 is outside of contact area, nodes 3 and 4 belong to the nonboundary point, and nodes 2 and 5 belong to the boundary point. For node 3, since its adjacent boundaries b23 and b34 are collinear, its normal direction is the common normal n3 of the two boundaries. For node 4, since its two adjacent boundaries b34 and b45 are not collinear, the normal direction of node 4 is the vector sum direction of boundaries b34 and b45, which can be obtained by (18)n4=n4,1+n4.2n4,1+n4,2Figure 4
Diagram of the wear direction determination of the brake pad node.Node 2 belongs to the boundary node, its adjacent boundaryb23 is in contact state, and adjacent boundary b12 is not in contact, so when wear occurs, node 2 moves along the direction n2 of the connecting line between node 2 and node 1. Therefore, through the analysis of the wear direction of the nodes, the mesh change process in the finite element analysis can be visually seen.


## 3.1. Calculation Model of the Brake Pad Wear

Due to extrusion and friction, the high temperature occurs on the friction pair at high-speed and heavy-load conditions, and there is serious wear on the friction contact. In 1953, the classical Archard wear theory was proposed by J. Archard [17]. The calculation equation is as follows:(1)V=KP·LHwhereV is the wear volume;P is the normal force of the contact surface;L is the relative sliding distance;H is the material hardness;K is the dimensionless wear coefficient. When the time increment is infinitesimal as dt, (1) can be extended to the differential form:(2)dVdL=K·PtHwhere dV is the instantaneous wear volume increment, dL is the instantaneous sliding distance, and Pt is the instantaneous normal interface contact force. Assuming that the wear depth increment on the microelement area ΔA is dh at time dt, the instantaneous wear volume increment can be expressed as(3)dV=ΔAdhwhere ΔA is the contact area of the brake disc and pad.Substituting (3) into (2), and it can be expressed as(4)dhdL=K·pHwhere p is the contact pressure at the contact microelement area ΔA, p=Pt/ΔA. Since the relative sliding distance L is the integral of the speed versus v timet, (4) can be rewritten as(5)dh=K·p·vHdt where the independent variables p and v of theoretical calculation are usually constant.However, under the actual high-speed and heavy-load braking conditions, the contact surface of any friction pair is rough. The actual contact area is related to the micromorphology of the contact surface. The stress value of every node on the contact interface is closely related to the wear depth and wear state of contact surface. The stress value changes with the wear depth change of each node on the contact surface, leading to the change wear degree of contact surface. Similarly, the high speed aggravates the friction of the contact pair, and a large amount of frictional heat is generated, and the friction material structure is changed, so does the hardness. The relationship between hardness and temperature of the material is as follows [18]:(6)H=const·exp⁡αθwhere α is a constant and θ is contact temperature.Wear is affected by the hardness of the friction material, and the change of temperature could affect the hardness of the friction material. Especially under high-speed and heavy-load braking conditions, the change of temperature is an important factor. Simultaneously, the virtual simulation software needs to calculate the relative contact speed, pressure, and temperature. However, the wear factors are considered distance, pressure, and material hardness in the original Archard wear calculation model. Therefore, the classical Archard wear model is no longer applicable for the simulated wear depth of a certain contact node. The Archard model is modified according to actual braking process. The contact pressurept, relative sliding velocity vt, and interface contact temperature θt are considered as influencing factors. The specific correction equation is as follows:(7)dht=K·pt·vtconst·exp⁡α/θtdtThe classical Archard wear equation is usually used to calculate the wear value of the relative rectilinear motion of two objects. However, when the brake disc and the brake pad of high-power disc brake are worn, the brake disc is in a state of rotation. The relative sliding speed of the contact interface is the tangential speed. Decompose the relative sliding tangential velocity:(8)vt=ωt·rwhere ωt is the relative sliding angular velocity and r is the friction radius of the brake pad. Substituting (8) into (7), it can be expressed as (9)dht=K·pt·ωtconst·exp⁡α/θt·rdtThe integral of (9) for time t in one braking time (0,t0) is expressed as(10)ht=K·r·∫0t0pt·ωtconst·exp⁡α/θtdtEquation (10) is a continuous integral solution. However, finite element analysis requires step-by-step solution in virtual simulation. So, the solution of (10) is very difficult because the variable curve of the contact node is very complicated. For the convenience of calculation, the continuous wear value is discretized by the discrete method: a finite small-time increment Δt is selected, and the corresponding wear depth increment is Δh. It is considered that the contact pressure pt, relative sliding angular velocity ωt, and contact temperature θt do not change large during time increment Δt, and the instantaneous values of pt, ωt, and θt are taken; then, Equation (9) becomes(11)Δht=K·r·pt·ωtconst·exp⁡α/θt·ΔtSince the wear of the brake interface is not evenly distributed between the brake disc and pad, the wear volume of the brake pad is solved by discrete method.As shown in Figure2, assuming that the unit friction radius increment is Δr within the time increment Δt, the unit microelement wear area can be expressed as(12)δAt=πr+Δr2-πr2·Δφ2πwhere Δφ is radians increment, Δφ=ωt·Δt. The unit wear volume of the brake pad within the time increment Δt is(13)ΔVt=δAt·ΔhtFigure 2
Calculation model of microelement wear area of the brake pad.Substituting (11) and (12) into (13), it can be expressed as(14)ΔVt=K·Δr+2r·r·Δr2·pt·ωt2const·exp⁡α/θt·Δt2When the disc brake is braking, the brake pad is considered as stationary state. There is wear on the brake pad, and the wear depth increment isΔh in Δt on the unit microelement contact area δA. The brake interface has different wear degrees with the change of the friction factor, and there is a feedback on the friction factor that the wear causes a change in the contact condition. The Euler integral method is used to calculate the wear by computer. The Euler method is a method of changing the differential equation of continuous variables to the difference equation of discrete variables. The numerical calculation is simple and easy, and the numerical convergence is good.In time incrementΔt, the contact pressure pt, relative sliding angular velocity ωt, and contact temperature θt are assumed to be constant. The wear depth increment Δht is obtained by Equation (11). The values of interface contact pressure pt, relative sliding angular velocity ωt, and contact temperature θt after wear can be obtained by the finite element method. Then the wear depth Δht can be calculated and the geometric mode is changed. Such loop iterations calculating the final accumulated wear value of the brake pad wear are obtained. The calculation method is as follows.Assuming that the contact node of the brake disc and the brake pad isi, i=1,2,…,N, and the integral step of the explicit Euler integral isj,j=1,2,…,M, then the contact pressure is pt(i,j), the relative sliding angular velocity is ωt(i,j), the contact temperature is θt(i,j), the wear depth is Δht(i,j), and the wear volume is ΔVt(i,j). The total wear depth h(i,j) and volume V(i,j) of braking at once of the brake pad can be expressed as(15)hi,j=∑j=1mΔht(16)Vi,j=∑j=1mΔVtThen the wear volume of the brake pad during the single braking of the disc brake can be expressed as(17)V=∑i=1nVi,jAccording to (17), the quantitative results of the brake pad wear after braking can be obtained. The process consists of two parts: one is to intercept and output the speed, stress, and temperature data in the wear stage from the time history curves of the contact point; the other is to divide the speed, stress, and temperature data and substitute these data into the equations to solve, as shown in Figure 3. DEFORM software has a special command to control the calculation of wear depth. Equation (5) can be added to the simulation program by compiling method to calculate the wear depth.Figure 3
Flow chart of wear calculation.


## 3.2. Determination of Wear Direction on Brake Pad Node

Affected by friction parameters, the surface roughness of contact surface after braking is different. There are two cases of the brake disc and the brake pad contact node: the boundary node at the edge of the contact surface and the nonboundary node located inside the contact surface. The wear direction of the nonboundary node can be determined by the normal of the contact node, and the wear direction of the boundary node is along the surface of the wear object. For the structured mesh, the connecting line direction of the nodes corresponding to their thickness direction is taken as the wear direction of point. As shown in Figure4, the wear contact area is indicated by dashed line, the nodes 2, 3, 4, and 5 are in the contact area, node 1 is outside of contact area, nodes 3 and 4 belong to the nonboundary point, and nodes 2 and 5 belong to the boundary point. For node 3, since its adjacent boundaries b23 and b34 are collinear, its normal direction is the common normal n3 of the two boundaries. For node 4, since its two adjacent boundaries b34 and b45 are not collinear, the normal direction of node 4 is the vector sum direction of boundaries b34 and b45, which can be obtained by (18)n4=n4,1+n4.2n4,1+n4,2Figure 4
Diagram of the wear direction determination of the brake pad node.Node 2 belongs to the boundary node, its adjacent boundaryb23 is in contact state, and adjacent boundary b12 is not in contact, so when wear occurs, node 2 moves along the direction n2 of the connecting line between node 2 and node 1. Therefore, through the analysis of the wear direction of the nodes, the mesh change process in the finite element analysis can be visually seen.


## 4. Establishment of Finite Element Model for Brake Pad Wear

To study the friction and wear characteristics of the brake pad during the braking process of high-power disc brake, it is necessary to establish a friction heat generation model and then the wear can be researched deeply. There are some assumptions as follows.(1) The contact interface of the friction pair is an ideal plane.(2) The friction condition accords with Coulomb’s law and the friction factor is constant during the disc braking.(3) The friction heat generated on the inner and outer sides of the brake pad is equal, so only one side of the brake disc is considered.(4) The instantaneous temperature of the corresponding point on the contact area of the brake disc and the brake pad is equal.(5) Assume that the pressure is evenly distributed on the brake pad.(6) The material of the brake disc and the brake pad is an isotropic material. Due to the short emergency braking time, the thermal property parameters of the material do not change with temperature.The model of brake disc and the brake pad is shown in Figure5. S1, S2, S3, and S4 are the upper surface, the lower surface, the surface of the outer circle side, and the surface of the inner circle side, respectively; A1, A2, and A3 are the wear surface of the brake pad, the side surface of the brake pad, and the upper surface of the brake pad, respectively; R1 and R2 are the inner and outer radius of the brake pad, respectively; R3 and R4 are the inner and outer circle radius of the brake disc, respectively; D1 and D2 indicate the thickness of the brake pad and the brake disc, respectively; φ is the wrap angle of the brake pad. The values are shown in Table 1.Table 1
The parameters of brake disc and brake pad.
Parameters R 1/(mm) R 2/(mm) R 3/(mm) R 4/(mm) D 1/(mm) D 2/(mm) φ Value 245 365 100 400 26 20 36°Figure 5
Diagram of the brake disc and the brake pad model.The results show that the stress-strain relationship of materials is greatly affected by factors of strain rate and temperature during plastic deformation. In order to simulating the braking process of the friction pair material accurately, a reasonable model is needed to describe the functional dynamic behavior of the material. When materials are subjected to dynamic loading conditions, a wide range of strains, strain rates, temperatures, and pressures may be experienced. Therefore, it is important that the effects of each variable be properly assessed, rather than assuming all distinguishing characteristics are due to strain rate alone [19].The Johnson-Cook model can reflect the strain rate and temperature rise softening effect well and is currently widely used in finite element simulation. The Johnson-Cook model is a product relationship that describes the relationship between strain effect, strain rate effect, and temperature effect. The specific expression is [20]:(19)σe=A+Bεepn1+Cln⁡εepεo1-T-TroomTmelt-Troommwhere σe is the equivalent flow stress, εep/ε0 is the relative equivalent plastic strain rate, εep is the equivalent plastic strain, and ε0 is reference plastic strain rate; the material constantsA,B,C,n, and m are the yield stress, hardening modulus, material strain rate strengthening parameter, hardening index, and thermal softening coefficient, respectively. Troom is the room temperature and Tmelt is the melting point of the material. The specific parameters of the brake disc and the brake pad material are shown in Tables 2 and 3.Table 2
Material parameters of the brake disc and the brake pad.
Material parameters Density/(kg/m3) Thermal conductivity/[W/(m·K)] Elastic modulus/(GPa) Poisson’sratio Linear expansion coefficient/(10−5) Specific heat capacity/[J/(kg·K)] Brake pad 5250 400 180 0.3 1.11 436 Brake disc 7850 48 204 0.31 0.95 480Table 3
Material constitutive parameters of the brake disc and the brake pad.
Constitutive parameters A B C n m Value 90 292 0.025 0.31 1.09The solid model is built by Pro/E according to the model of brake disc and the brake pad, as shown in Figure6(a). The finite element analysis of the solid model is then performed using the finite element analysis DEFORM software. The brake pad is rigid body and the brake disc is plastic. The mesh of the brake disc and the brake pad is meshed by the free mesh module. The number of elements of the brake disc is 58591, and the number of nodes is 14138; the number of elements of the brake pad is 7703, and the number of nodes is 1898. The contact between the brake disc and the brake pad is set to point contact, as shown in Figure 6(b).Figure 6
Finite element model of brake disc and brake pad.
(a)
Solid model (b)
Grid modelBased on the adaptive meshing technology of Deform-3D software, the deformation volume of the brake disc and the brake pad model is compensated automatically by using the tetrahedral mesh. The corresponding mesh encryption in the contact area of the brake friction pair ensures the calculation accuracy and improves the calculation efficiency. According to the high-speed and heavy-load conditions, the brake pad is considered as stationary, and the brake disc is rotated anticlockwise. The brake pad is clamped by the brake caliper, a fixed constraint inx and y directions is applied to the brake pad on A2; the brake pad is subjected to the hydraulic piston-rod, assuming that the pressure is evenly distributed on the brake pad upper surface A3. It can be expressed as(20)σz=pupx=upy=0z=D1,R1≤r≤R2where σz is the pressure of the brake pad in z direction;p is the initial braking load; upx, upy are the displacements of the brake pad that may occur in x and y directions, as shown in Figure 7. The lower surface S2 of the brake disc is axially fixedly constrained in z direction. There can be expressed as(21)udz=0z=0,R3≤r≤R4where udz is the displacement of the brake disc in z direction. Since the inner hole of the brake disc is connected to the brake shaft, a fixed constraint in thez-axis direction is applied to the inner circular side, and a rotational constraint of an angular velocity of ωt is applied to simulate the decelerating motion of the brake disc. It can be expressed as(22)ω=ωtudz=00≤z≤D2,r=R3where ω is the rotational angular velocity of the brake disc and udz is the displacement of the brake disc in z direction, as shown in Figure 8.Figure 7
Diagram of the brake pad boundary conditions.Figure 8
Diagram of the brake disc boundary conditions.According to assumption (6), the heat exchange coefficient of the brake disc and the brake pad interface selected 45N/sec/mm/C as a constant. The ambient temperature is 20°C; the shear failure model and the tensile failure model are selected. And the wear Equation (5) is used to calculate the wear depth of the brake pad by program, based on the Archard wear correction equation. Braking load of 13000N, initial braking speed of 1000r/min, and braking time of 24.98s are selected, and the finite element analysis is carried out.


## 5. Analysis of Simulation Results of the Brake Pad Wear

### 5.1. Simulation Analysis of the Brake Pad Wear in Single Braking

The wear process of the brake pad is an accumulation, and the results of wear on the surface of the brake pad under different steps are shown in Figure9. The brake pad wear is mainly affected by the friction force. According to the friction direction of the brake pad in Figure 9(a), the left edge of the brake pad is defined as a friction inlet, and the right edge is defined as a friction outlet.Figure 9
Nephogram of the brake pad wear depth.
(a)
Step 1 (b)
Step 10 (c)
Step 200 (d)
Step 500 (e)
Step 800 (f)
Step 1000According to the wear nephogram of the brake pad, it can be seen that the wear distribution of the brake pad during the braking process is uneven, and the wear area changes with time. Throughout the whole wear process, there is a significant difference in the wear degree between the friction inlet and the friction outlet of the brake pad. Both ends of the edge of the brake pad are affected seriously by tensile stress and compressive stress on the friction inlet and outlet, respectively. Due to the rotary motion of the brake disc, there is a linear speed difference in the radial direction of the brake disc, and the outer edge of the brake pad has a large line speed and wear, while the inner edge wear of the brake pad is weak.The data pointsP1-P15 uniformly distributed on the brake pad are extracted from Figure 10, and the simulated wear depth of points is extracted according to the simulation results of the data points. The wear depth curves of the brake track point are drawn as shown in Figure 11. The wear depth is represented by points P1-P15 of the curves from the friction inlet to the friction outlet. To clearly describe the wear condition of the brake pad, let points P1, P6, and P11 belong to the friction inlet region, and points P5, P10, and P15 belong to the friction outlet region point; the others belong to the friction intermediate region. The wear of the friction inlet of the brake pad is composed of two parts. One part of wear is caused by extrusion caused by the relative movement of the brake disc and the brake pad. The elements of the brake pad and the brake disc are squeezed against each other, so that the surface of the brake disc is not flat due to deformation of the mesh element. The other part is the effect of the braking friction on the rough surface. There will be rough peaks on the surface of the deformation of the brake disc. And the rough peaks are squeezed during the relative movement, causing the material to undergo shear deformation and wear. The combination of the two parts aggravates the deformation of the material. The interface contact pressure increases and the local temperature rises, so that the wear is severe. And the wear depth at the edge of friction inlet is relatively large. Because the friction intermediate region is far away from the friction edge and the pressing force is small, the material deformation is not obvious, and the friction heat is low, and then the wear degree is small. In the middle area of the brake pad, the wear depth increases slowly firstly and then rises sharply with the change of temperature and pressure. Due to the heat conduction of the brake disc, the friction outlet temperature of the brake pad is high, and the wear is mainly adhesive wear. The friction material transfers adhesively so that the friction surface is rough.Figure 10
Nephogram of the brake pad point tracking.Figure 11
Chart of the brake pad point tracking wear curves.The severe wear of the brake pad during braking only occurs in local areas. Figure12 shows the three-dimensional wear profile of the brake pad at the 1000th step. As shown in Figure 12(a), the brake pad is serious at the edge of the friction outlet; at this time the maximum wear depth is 0.0684mm. The severe wear area accounts for a small part of the total area of the brake pad, and the wear depth of other part area is low. The surface topography does not change obviously. To clearly analyze the change of surface topography, half of the maximum wear depth 0.0137mm, mesoscopic size of wear depth 0.005mm and 0.001mm of this time are selected respectively to limit the maximum wear. And the surface topography is output and observed from different wear levels as half of the maximum wear depth 0.0137mm, mesoscopic size of wear depth 0.005mm and 0.001mm. When the maximum wear depth is limited to 0.0137mm, the wear depth of the friction outlet of the brake pad changes obviously. This is because there is no material back up at the friction outlet. The material is easily broken and fractured during braking, causing severe wear as shown in Figure 12(b). The closer it is to the friction outlet, the greater the wear degree is. It can also be seen from Figures 12(c) and 12(d) that the surface roughness is large from the friction outlet to the intermediate area, the local wear is severely at the friction outlet.Figure 12
Nephogram of wear profile of the brake pad at different maximum wear depths.
(a)
0.0684mm (b)
0.0137mm (c)
0.005mm (d)
0.001mmBraking parameters are the keys to ensuring brake safety on the premise of braking efficiency. Proper selecting of braking parameters not only saves energy, but also saves material losses caused by wear. Therefore, it is necessary to study the influence of braking parameters on the brake pad wear. The braking load and initial braking speed play important roles in the brake pad wear during braking process. The single variable method is used to compare the brake pad wear under different working conditions.


### 5.2. Influence of Braking Load on the Brake Pad Wear

Under the conditions of initial braking speed is 1000r/min and friction coefficient of contact surface is 0.3, the brake pad wear with brake loads of 13000N, 17000N, and 21000N is analyzed by finite element method. The nephogram of the brake pad at the end of braking is shown in Figure13. According to the simulation results, the maximum wear depth of the corresponding steps can be extracted. Figure 14 shows the number of simulation steps is as the horizontal axis, and the maximum wear depth is as the vertical axis and the comparison curves of the maximum brake pad wear depth under different braking loads.Figure 13
Nephogram of the brake pad wear with different braking loads.
(a)
Braking load 13000N (b)
Braking load 17000N (c)
Braking load 21000NFigure 14
Chart of the brake pad wear depth with different braking loads.The wear distribution of the brake pad under different loads is basically the same. The maximum wear depth is 6.4 × 10−2mm when the number of simulation steps is the 1000th step and the braking load is 13000N. The maximum wear depth is 7.34 × 10−2mm when the braking load is 17000N, and the maximum wear depth is 8.09 × 10−2mm when the braking load is 21000N. Friction always occurs at a part of the contact peak, and the number of contacts point and the size of each contact point increase with load. Therefore, the friction is affected by load through the contact area size and deformation state. And then the friction affects the wear of the material. The increase of braking load directly increases the contact pressure of the friction pair. The interface contact area becomes large, forcing the friction material to deform and aggravating the wear of the brake pad. Figure 14 shows the change in the amount of the brake pad wear under different braking loads. In the 200th step of the early wear stage of the brake pad, the wear is in a sharp rise stage, and the effect of braking load on the wear is small. In the later wear stage from the 200th step to the 1000th step, the slope of the wear curve remains basically the same, and the accumulation of wear increases steadily. However, the maximum amount of wear between the different loads is obviously different and the accumulation of wear difference becomes large.


### 5.3. Influence of Initial Braking Speed on the Brake Pad Wear

It is planned to the braking load 17000N and the friction coefficient 0.3 of the contact surface. Compared with the brake pad wear degree of initial braking speeds of 800r/min, 1000r/min, and 1200r/min, respectively, the distribution trend is shown in Figure15. In order to analyze the wear change of the brake pad accurately, the brake pad wear simulation results can be obtained through postprocessing. The comparison curves of the maximum wear depth of the brake pad under different initial braking speeds are shown in Figure 16.Figure 15
Nephogram of the brake pad wear with different initial braking speeds.
(a)
Initial braking speed 800r/min (b)
Initial braking speed 1000r/min (c)
Initial braking speed 1200r/minFigure 16
Chart of the brake pad wear depth with different initial braking speeds.Figure15 shows the wear distribution of the brake pad at different initial braking speeds at the 1000th step. The maximum wear depth at the initial braking speed of 800r/min is 6.71 × 10−2mm, and the radial wear of the brake pad is unevenly transitioned from the inner circle region to the outer circle region. When the initial braking speed is 1000r/min, the maximum wear depth is 7.34 × 10−2mm. When the initial braking speed is 1200r/min, the radial wear of the brake pad changes uniformly, and the maximum wear depth is 8.25 × 10−2mm. Generally, the surface layer heating, deformation, chemical changes, and wear are caused by the relative sliding speed. The relative sliding speed affects the friction force through the temperature condition of the brake pad. The change of heating and temperature can change the property of the surface layer and the surface interaction and failure conditions during friction. Therefore, the wear degree of the brake pad is different. The initial braking speed determines the relative sliding speed during the braking process. Large relative sliding speed increases the extrusion force and shear force of the rough surface during friction, leading to the increase of strain, stress value, and more serious wear of the brake pad. In Figure 16, the horizontal axis represents the number of simulation steps, and the vertical axis represents the maximum amount of wear. The wear curves show in the increase degree of maximum wear of the brake pad. The maximum wear depth at the initial braking speed of 1200r/min is generally greater than that at the initial braking speed of 1000r/min during braking. The maximum wear depth at the initial braking speed of 1000r/min is also greater than that at the initial braking speed of 800r/min. The difference of the maximum wear depth of the three conditions is relatively small in the early wear stage. The wear difference is large in the later wear stage, and the difference value is basically the same.


## 5.1. Simulation Analysis of the Brake Pad Wear in Single Braking

The wear process of the brake pad is an accumulation, and the results of wear on the surface of the brake pad under different steps are shown in Figure9. The brake pad wear is mainly affected by the friction force. According to the friction direction of the brake pad in Figure 9(a), the left edge of the brake pad is defined as a friction inlet, and the right edge is defined as a friction outlet.Figure 9
Nephogram of the brake pad wear depth.
(a)
Step 1 (b)
Step 10 (c)
Step 200 (d)
Step 500 (e)
Step 800 (f)
Step 1000According to the wear nephogram of the brake pad, it can be seen that the wear distribution of the brake pad during the braking process is uneven, and the wear area changes with time. Throughout the whole wear process, there is a significant difference in the wear degree between the friction inlet and the friction outlet of the brake pad. Both ends of the edge of the brake pad are affected seriously by tensile stress and compressive stress on the friction inlet and outlet, respectively. Due to the rotary motion of the brake disc, there is a linear speed difference in the radial direction of the brake disc, and the outer edge of the brake pad has a large line speed and wear, while the inner edge wear of the brake pad is weak.The data pointsP1-P15 uniformly distributed on the brake pad are extracted from Figure 10, and the simulated wear depth of points is extracted according to the simulation results of the data points. The wear depth curves of the brake track point are drawn as shown in Figure 11. The wear depth is represented by points P1-P15 of the curves from the friction inlet to the friction outlet. To clearly describe the wear condition of the brake pad, let points P1, P6, and P11 belong to the friction inlet region, and points P5, P10, and P15 belong to the friction outlet region point; the others belong to the friction intermediate region. The wear of the friction inlet of the brake pad is composed of two parts. One part of wear is caused by extrusion caused by the relative movement of the brake disc and the brake pad. The elements of the brake pad and the brake disc are squeezed against each other, so that the surface of the brake disc is not flat due to deformation of the mesh element. The other part is the effect of the braking friction on the rough surface. There will be rough peaks on the surface of the deformation of the brake disc. And the rough peaks are squeezed during the relative movement, causing the material to undergo shear deformation and wear. The combination of the two parts aggravates the deformation of the material. The interface contact pressure increases and the local temperature rises, so that the wear is severe. And the wear depth at the edge of friction inlet is relatively large. Because the friction intermediate region is far away from the friction edge and the pressing force is small, the material deformation is not obvious, and the friction heat is low, and then the wear degree is small. In the middle area of the brake pad, the wear depth increases slowly firstly and then rises sharply with the change of temperature and pressure. Due to the heat conduction of the brake disc, the friction outlet temperature of the brake pad is high, and the wear is mainly adhesive wear. The friction material transfers adhesively so that the friction surface is rough.Figure 10
Nephogram of the brake pad point tracking.Figure 11
Chart of the brake pad point tracking wear curves.The severe wear of the brake pad during braking only occurs in local areas. Figure12 shows the three-dimensional wear profile of the brake pad at the 1000th step. As shown in Figure 12(a), the brake pad is serious at the edge of the friction outlet; at this time the maximum wear depth is 0.0684mm. The severe wear area accounts for a small part of the total area of the brake pad, and the wear depth of other part area is low. The surface topography does not change obviously. To clearly analyze the change of surface topography, half of the maximum wear depth 0.0137mm, mesoscopic size of wear depth 0.005mm and 0.001mm of this time are selected respectively to limit the maximum wear. And the surface topography is output and observed from different wear levels as half of the maximum wear depth 0.0137mm, mesoscopic size of wear depth 0.005mm and 0.001mm. When the maximum wear depth is limited to 0.0137mm, the wear depth of the friction outlet of the brake pad changes obviously. This is because there is no material back up at the friction outlet. The material is easily broken and fractured during braking, causing severe wear as shown in Figure 12(b). The closer it is to the friction outlet, the greater the wear degree is. It can also be seen from Figures 12(c) and 12(d) that the surface roughness is large from the friction outlet to the intermediate area, the local wear is severely at the friction outlet.Figure 12
Nephogram of wear profile of the brake pad at different maximum wear depths.
(a)
0.0684mm (b)
0.0137mm (c)
0.005mm (d)
0.001mmBraking parameters are the keys to ensuring brake safety on the premise of braking efficiency. Proper selecting of braking parameters not only saves energy, but also saves material losses caused by wear. Therefore, it is necessary to study the influence of braking parameters on the brake pad wear. The braking load and initial braking speed play important roles in the brake pad wear during braking process. The single variable method is used to compare the brake pad wear under different working conditions.


## 5.2. Influence of Braking Load on the Brake Pad Wear

Under the conditions of initial braking speed is 1000r/min and friction coefficient of contact surface is 0.3, the brake pad wear with brake loads of 13000N, 17000N, and 21000N is analyzed by finite element method. The nephogram of the brake pad at the end of braking is shown in Figure13. According to the simulation results, the maximum wear depth of the corresponding steps can be extracted. Figure 14 shows the number of simulation steps is as the horizontal axis, and the maximum wear depth is as the vertical axis and the comparison curves of the maximum brake pad wear depth under different braking loads.Figure 13
Nephogram of the brake pad wear with different braking loads.
(a)
Braking load 13000N (b)
Braking load 17000N (c)
Braking load 21000NFigure 14
Chart of the brake pad wear depth with different braking loads.The wear distribution of the brake pad under different loads is basically the same. The maximum wear depth is 6.4 × 10−2mm when the number of simulation steps is the 1000th step and the braking load is 13000N. The maximum wear depth is 7.34 × 10−2mm when the braking load is 17000N, and the maximum wear depth is 8.09 × 10−2mm when the braking load is 21000N. Friction always occurs at a part of the contact peak, and the number of contacts point and the size of each contact point increase with load. Therefore, the friction is affected by load through the contact area size and deformation state. And then the friction affects the wear of the material. The increase of braking load directly increases the contact pressure of the friction pair. The interface contact area becomes large, forcing the friction material to deform and aggravating the wear of the brake pad. Figure 14 shows the change in the amount of the brake pad wear under different braking loads. In the 200th step of the early wear stage of the brake pad, the wear is in a sharp rise stage, and the effect of braking load on the wear is small. In the later wear stage from the 200th step to the 1000th step, the slope of the wear curve remains basically the same, and the accumulation of wear increases steadily. However, the maximum amount of wear between the different loads is obviously different and the accumulation of wear difference becomes large.


## 5.3. Influence of Initial Braking Speed on the Brake Pad Wear

It is planned to the braking load 17000N and the friction coefficient 0.3 of the contact surface. Compared with the brake pad wear degree of initial braking speeds of 800r/min, 1000r/min, and 1200r/min, respectively, the distribution trend is shown in Figure15. In order to analyze the wear change of the brake pad accurately, the brake pad wear simulation results can be obtained through postprocessing. The comparison curves of the maximum wear depth of the brake pad under different initial braking speeds are shown in Figure 16.Figure 15
Nephogram of the brake pad wear with different initial braking speeds.
(a)
Initial braking speed 800r/min (b)
Initial braking speed 1000r/min (c)
Initial braking speed 1200r/minFigure 16
Chart of the brake pad wear depth with different initial braking speeds.Figure15 shows the wear distribution of the brake pad at different initial braking speeds at the 1000th step. The maximum wear depth at the initial braking speed of 800r/min is 6.71 × 10−2mm, and the radial wear of the brake pad is unevenly transitioned from the inner circle region to the outer circle region. When the initial braking speed is 1000r/min, the maximum wear depth is 7.34 × 10−2mm. When the initial braking speed is 1200r/min, the radial wear of the brake pad changes uniformly, and the maximum wear depth is 8.25 × 10−2mm. Generally, the surface layer heating, deformation, chemical changes, and wear are caused by the relative sliding speed. The relative sliding speed affects the friction force through the temperature condition of the brake pad. The change of heating and temperature can change the property of the surface layer and the surface interaction and failure conditions during friction. Therefore, the wear degree of the brake pad is different. The initial braking speed determines the relative sliding speed during the braking process. Large relative sliding speed increases the extrusion force and shear force of the rough surface during friction, leading to the increase of strain, stress value, and more serious wear of the brake pad. In Figure 16, the horizontal axis represents the number of simulation steps, and the vertical axis represents the maximum amount of wear. The wear curves show in the increase degree of maximum wear of the brake pad. The maximum wear depth at the initial braking speed of 1200r/min is generally greater than that at the initial braking speed of 1000r/min during braking. The maximum wear depth at the initial braking speed of 1000r/min is also greater than that at the initial braking speed of 800r/min. The difference of the maximum wear depth of the three conditions is relatively small in the early wear stage. The wear difference is large in the later wear stage, and the difference value is basically the same.


## 6. Experimental Verification

### 6.1. Experimental Procedure

The wear test of the brake pad is carried out in a high-power wind turbine brake, as shown in the Figure17. The disc brake can be used for the braking performance test of high-speed and heavy-load conditions for high-power disc brake and could meet the requirements of the braking wear test in the emergency conditions. The brake disc is interconnected to the brake shaft by a keyway. There are some assumptions as follows. (1) When the drive shaft and the inertia flywheel are rotated to the set speed of 1000r/min, the brake disc is released from the control of the drive motor and the brake pad is loaded by hydraulic pressure. (2) Friction is generated to achieve braking of the brake disc due to the relative sliding of the brake disc and the brake pad.Figure 17
High-power wind turbine brake.The brake pad material is made of copper-based powder metallurgy and the brake disc material is Q345B. The material properties have the same characteristics in Table1. The size and installation position of the brake disc and brake pad on the test machine are consistent with the model of brake disc and the brake pad with Figure 5. Test condition parameters are shown in Table 4.Table 4
Test condition parameters.
Number of friction faces Moment of inertia/ (kg·m2) Ambient temperature/ (°C) Atmospheric intensity of pressure/ (KPa) Relative humidity Braking pressure/ (N) Initial braking speed/ (r/min) 1 700 20 101.3 37% 13000 1000Besides, in order to remove surface impurities, the surface of the brake disc and the brake pad need to be polished with sandpaper. There is also a micrometer for measuring the different positions of the brake disc and the brake pad to ensure that the two surfaces are smooth enough to produce a good fit.


### 6.2. Results and Discussion

In order to verify the accuracy of simulation, the finite element wear depth results (Figure10) are compared with the actual wear of the brake pad under the same operating conditions in experiments (Figure 18). Points Q1-Q15 at the corresponding positions on Figure 18 are measured by 1:1000mm digital dial gauge, and each position is measured three times to take the average values as the wear depth of points Q1-Q15. The results comparison of simulation and experimental wear depth are drawn as shown in Figure 19.Figure 18
Nephogram of the brake pad experimental measuring point position.Figure 19
Comparison of the brake pad simulation and experimental wear depth.
(a)
Simulation wear depth (b)
Experimental wear depthIn the actual friction and wear process, the friction heat of the surface material rises quickly with the braking process. High temperature reduces the hardness of the material, promoting the deformation of the brake disc and the brake pad. The copper-based material will be softened with the temperature rising rapidly. Softening of the copper-based material leads to a decrease in particle holding ability, increasing the surface wear of the brake pad, as shown in Figure18. Figure 19 shows the wear depth in the simulation and experimental results of the brake pad. The x axis represents the lateral distribution of the brake pad, and the y axis represents the longitudinal distribution. Comparing the simulated and experimental results of wear depth, although the values between the brake disc and the brake pad are very different, the wear distribution trend at different locations is still roughly the same. The main reason for the difference between the two values is the difference of braking time. In simulations, due to the limited number of simulation steps, the simulated braking time is much shorter. But in experiments, to facilitate the observation of wear state, the actual braking time is long. Comparing the longitudinal distribution of the simulated and experimental results, the outer circle region and inner circle region of the friction inlet wear value are larger than those of the middle region results. This is because stress concentration occurs without backing up by the side material in the outer circle region and inner circle region. The wear depth at the friction outlet increases from the inner circle region to the outer circle region, because the outer circle region has a higher frictional line speed than the inner circle region, and the temperature of the outer circle region is high, the corresponding wear is also large. Comparing the lateral distribution of the simulation and experimental wear, there is large wear at the friction inlet. The wear shows as a rising trend from the intermediate area to the wear outlet. Due to the short simulation time, the brake pad wear depth far away from the wear outlet is small, and the difference of the wear in the middle area is large. However, the surface wear is relatively uniform and the wear difference is small after a period of wear.


## 6.1. Experimental Procedure

The wear test of the brake pad is carried out in a high-power wind turbine brake, as shown in the Figure17. The disc brake can be used for the braking performance test of high-speed and heavy-load conditions for high-power disc brake and could meet the requirements of the braking wear test in the emergency conditions. The brake disc is interconnected to the brake shaft by a keyway. There are some assumptions as follows. (1) When the drive shaft and the inertia flywheel are rotated to the set speed of 1000r/min, the brake disc is released from the control of the drive motor and the brake pad is loaded by hydraulic pressure. (2) Friction is generated to achieve braking of the brake disc due to the relative sliding of the brake disc and the brake pad.Figure 17
High-power wind turbine brake.The brake pad material is made of copper-based powder metallurgy and the brake disc material is Q345B. The material properties have the same characteristics in Table1. The size and installation position of the brake disc and brake pad on the test machine are consistent with the model of brake disc and the brake pad with Figure 5. Test condition parameters are shown in Table 4.Table 4
Test condition parameters.
Number of friction faces Moment of inertia/ (kg·m2) Ambient temperature/ (°C) Atmospheric intensity of pressure/ (KPa) Relative humidity Braking pressure/ (N) Initial braking speed/ (r/min) 1 700 20 101.3 37% 13000 1000Besides, in order to remove surface impurities, the surface of the brake disc and the brake pad need to be polished with sandpaper. There is also a micrometer for measuring the different positions of the brake disc and the brake pad to ensure that the two surfaces are smooth enough to produce a good fit.


## 6.2. Results and Discussion

In order to verify the accuracy of simulation, the finite element wear depth results (Figure10) are compared with the actual wear of the brake pad under the same operating conditions in experiments (Figure 18). Points Q1-Q15 at the corresponding positions on Figure 18 are measured by 1:1000mm digital dial gauge, and each position is measured three times to take the average values as the wear depth of points Q1-Q15. The results comparison of simulation and experimental wear depth are drawn as shown in Figure 19.Figure 18
Nephogram of the brake pad experimental measuring point position.Figure 19
Comparison of the brake pad simulation and experimental wear depth.
(a)
Simulation wear depth (b)
Experimental wear depthIn the actual friction and wear process, the friction heat of the surface material rises quickly with the braking process. High temperature reduces the hardness of the material, promoting the deformation of the brake disc and the brake pad. The copper-based material will be softened with the temperature rising rapidly. Softening of the copper-based material leads to a decrease in particle holding ability, increasing the surface wear of the brake pad, as shown in Figure18. Figure 19 shows the wear depth in the simulation and experimental results of the brake pad. The x axis represents the lateral distribution of the brake pad, and the y axis represents the longitudinal distribution. Comparing the simulated and experimental results of wear depth, although the values between the brake disc and the brake pad are very different, the wear distribution trend at different locations is still roughly the same. The main reason for the difference between the two values is the difference of braking time. In simulations, due to the limited number of simulation steps, the simulated braking time is much shorter. But in experiments, to facilitate the observation of wear state, the actual braking time is long. Comparing the longitudinal distribution of the simulated and experimental results, the outer circle region and inner circle region of the friction inlet wear value are larger than those of the middle region results. This is because stress concentration occurs without backing up by the side material in the outer circle region and inner circle region. The wear depth at the friction outlet increases from the inner circle region to the outer circle region, because the outer circle region has a higher frictional line speed than the inner circle region, and the temperature of the outer circle region is high, the corresponding wear is also large. Comparing the lateral distribution of the simulation and experimental wear, there is large wear at the friction inlet. The wear shows as a rising trend from the intermediate area to the wear outlet. Due to the short simulation time, the brake pad wear depth far away from the wear outlet is small, and the difference of the wear in the middle area is large. However, the surface wear is relatively uniform and the wear difference is small after a period of wear.


## 7. Conclusions

This work has focused on an investigation and comparison of the wear progression and wear mechanism of the brake pad in the high-speed and heavy-load conditions. The followings are the key conclusions drawn from this study.(1) The wear of the brake pad is a cumulative process, and the wear depth of the brake pad increases quickly and then slowly. The friction inlet and outlet edge regions of brake pad are extruded during braking, which is severely worn compared to the middle of the brake pad. Compared with the experimental results, it is the same trend that the proposed simulation model is in different parts. So, the model validity is verified.(2) The load affects the wear of the brake pad by affecting the contact state of interface, and the increase of brake load aggravates the wear of the brake pad. When the braking load is increased from 13000N to 17000N, the maximum wear depth of the brake pad is 8.09 × 10−2mm. The relative sliding speed is determined by initial braking speed. As the initial braking speed increases, the frictional heat caused by high speed accelerates the brake pad wear. It is difficult to brake in the high initial braking speed, and the brake pad wear is serious. When the braking load is 21000N, the initial braking speed is 1200 r/min, and the maximum wear depth is 8.25 × 10−2mm.



---

*Source: 6250694-2019-07-14.xml*